KEER2014, LINKÖPING | JUNE 11-13 2014
INTERNATIONAL CONFERENCE ON KANSEI ENGINEERING AND EMOTION RESEARCH
Influence of Fiber’s Surface Morphology Change on
Anti-pilling Performance of Woolen Knitted Fabric
Masukuni Mori1, Takako Fujiumoto2 and Machiko Murakami3
1Mori Consultant Engineering Office Japan,firstname.lastname@example.org
2Hokkaido University of Education,.Japan, email@example.com
3Gifu City Women’s Junior College,Japan
Abstract: Although the main factor controlling pill generation at the time of wearing wool knitted
articles is the knitting structure of the raw material; the strength of yarn, the number of twist of yarn,
the fabric design, the gauge number and so on, it is influenced also by the dyeing / finishing
method of the knitted fabric after knitting as well.
In this paper, the influence of change in surface morphology of raw material fiber on pill generation
is investigated (along with mechanical and physical properties of fabrics). Fabric samples are
treated with several physicochemical processing. The difference in condition of scales and the
relation with pill generation were discussed and clarified. The plain knit wear is widely used for
sportswear and child’s underwear subjected to high activity. Such clothing necessitates
comfortable and soft touch and besides the surface of the clothing must be kept smooth and
anti-pilling condition. These requirements are hopeful for comfortable clothing life. Thus, the
present paper is believed to be a suitable topic relevant to Kansei Engineering.
Keywords: Pilling, Surface morphology, Wool-Knit, Physicochemical treat.
The generation of the pill at the time of wearing wool knitted fabrics mainly originates from
properties of the raw material, the number of twist of the yarn, the fabric design and the gauge
number, and others. But sometimes such a design is unwillingly employed because of aesthetic
necessity and soft handle. For child clothes and sportswear subjected to high activity, anti-pilling
fabric are required. The pilling phenomenon is largely developed when the yarn as the raw material
is long and tough, and the structure of knit composed of yarns with low twist density is coarse. The
generation of the pill on the wool knitted fabrics is also influenced by the post processing of dyeing
and finishing. In our preceding work [(Mori et al 2013), we discussed about the influence of dyeing
and finishing processes on the performance of woolen and worsted fabrics. And it was confirmed
that handling and feeling of the fabrics could be modified by physicochemical finishing processes.
In the present work, first the generation of the pill was investigated for wool knitted fabrics
subjected to 4 kinds of post physicochemical processing such as Chlorination (Breck et
al ,1989), NARS shrink-proof (Cadamone et al,2004), Argon low temperature plasma(Mori et
al.2006) , and Polyuretane resin treatment and so on in which anti-pilling function is expected to
be endowed. Next, the relation of the unevenness on the fiber surface, i.e. the state of scale height
to the pilling nature was investigated in that the generation of pilling was ascribed to entanglement
of fluffs on fabric surface. The state of the pilling was comparatively evaluated from 3 kinds of
information that the number of pills on a prescribed area of the test fabric after pilling test, the
number of pills dropped out and the size of the pill. The 3 kinds of information here are (ⅰ)
Five-rank evaluation based on JIS-1076-1992, (ⅱ) Average number of pills generating on a area
of 12×10 cm2 of the test fabric, and (ⅲ) number of pills dropped out into the box of tester. AS a
result, high correlativity of the scale height with number of Pills (R2=0,71)was found out. This
means that the generation of pilling is easily brought about by large difference between low and
high scales. To further confirm this correlation, the scale height must be measured, and the
measurement by AFM( Atomic Force Microscope)is now under consideration.
The sample used is composed of merino wool yarns of 20.1～21.0 µm in diameter 2/60 (33.3
dtex) . The structure is plain weave. As to the count of twist, lower twist is set 685Z, while upper
twist is set 685S. Coarse density is 153/10cm and wale density is 134/10cm, respectively, and
weigh is 178g/cm2. The physical properties of materials are summarized in Table 1.
Table 1: Physical properties of materials
Materials Yarn Knitted Fabric
Count Twist Density(/10cm) Weight(g/cm2)
33.3dtex 685Z/685S 153 134 178
2.2. Details of finishing processes
Samples are classified into 5 fabrics. 4 kinds of physicochemical treatments were subjected to
Sample 1: Grey fabric; Knit wool fabric described in 2.1
Sample 2 in which chlorination treatment was practiced on sample 1 and scales on the surface
of wool were removed.
Sample 3 in which surface modification by NARS processing was subjected to sample 1.
Sample 4 in which aqueous emulsion type resin processing was practiced on sample 1.
Sample 5 in which Argon Low Temperature Plasma exposure was subjected to sample 1.
2.2.1. Chlorination treatment
Fabric samples placed in a dyeing bath were dipped in water at 20 to 25 ℃ under a liquor to
wool ratio of 20 : 1, and the amount corresponding to 0.05% non-ionic surfactant was added as a
penetrating agent to the dyeing bath. The dyeing bath was stirred until the fabric samples were
perfectly soaked in it. Then, solutions of 3.0% (o.w.f. as active chlorine) DCCA and 5.0% (o.w.f.)
sodium pyrophosphate (Na2P2O7・10H2O) were added, further acetic acid was added to adjust pH
within the range of 5.5 to 6.0, and the resultant solution was maintained for a period of 20 min at
this temperature. The temperature of the solution was then raised to 35 ℃ in 10 min, and
maintained for 20 min. 6% (o.w.f.) sodium hydrogen sulfite (NaHSO3) was further added, and after
the temperature of solution had been raised to 60 ℃ , the solution was maintained at this
temperature for 10 min. The treated fabrics were rinsed and dried by air. The fabric samples
treated with such chlorination processing were subjected to property measurements.
2.2.2. NARS shrink-proof processing
According to a modified method of the procedure described in U.S. Agricultural Research
Service (Wyndmoor, PA 19038), treatments to wool fabric were carried out at conditions of pH 10.2,
30 ℃, period of 30 min and liquor to wool ratio of 20 :1 using a laboratory dyeing machine
containing 1 g/L Ttriton X-114, 3 g/L NaOH, 1 g/L gluconic acid, 3 g/L dicyandiamide, and 12 g/L
H2O2 (35%). After such treatment, the fabrics were rinsed until reaching neutral pH. Successively
the treatment by enzyme was carried out at 50 ℃ and pH 6.0 for 40 min in a bath dissolving
1.5g/L triethanolamine (TEA), 1g/L Triton X-114, 1.5% (o.w.f.) Na2SO3 and Esperase 8.0LTM
(Novoenzymes, North America, Flaklington, NC). After the treatment, the enzyme was deactivated
at the conditions of 80 ℃ and period of 10 min. The fabrics were rinsed and dried by air.
2.2.3. Water soluble polyurethane resin treatment
As for sample, aqueous emulsion type resin Supeperflex R 5002 is in a state of 5 % solution.
Pad was extracted, and it was cured during 1 min at 130 ℃ after the drying process.
2.2.4. Argon low temperature plasma treatment
Plasma reactor used is a type DSSO-422 (Daia Sinku Co., Ltd.). The discharge frequency was
fixed at 13.56 MHz. Plasma treatment was carried out by the following procedures. The sample
was placed in the reactor, and the reactor was evacuated to 0.001 Torr (0.13 Pa). Then argon (Ar)
was fed into it at a volumetric flow rate of 10 mL/min. The electric power for plasma discharge was
fixed at 100 W. The internal pressure of the reactor was maintained at 0.1 Torr (13.3 Pa) during a
plasma-treatment time of 300 s. The treated fabric samples were finally rinsed with water and dried
by air, and then they were subjected to property measurements.
2.3. Pilling test method
Pilling conditions for treated and untreated sample fabrics are based on the JIS L-1076-1992
(ISO 12945-1) method. The measurements for the treated fabrics were compared with the
measurement for the untreated fabric. According to the method, the ranking from the first to the
fifth rank is determined. To determine more accurate ranking of the fabric, in this study, the
information on both the number of pills in the 12×10cm area and the number of the pills
dropped out was employed.
2.4. Breaking strength
Items of breaking strength, elongation for an untreated fabric and 4 kinds of treated knit fabrics
were measured based on JIS L-1095 by means of tension tester AG-IS 10KN (Shimadzu
Manufacturing Co. Ltd., Japan). The average breaking strength (N) and elasticity (%) were
determined under the conditions of number of samples = 50, sample length and width = 200 mm
and 50 mm, respectively, initial load = 0.05N, and pulling speed = 200 mm/min.
2.5. Bursting strength
The bursting test was executed by means of constant elongation method based on
JIS-L1096-8.16. First, five test pieces of 8 cm diameter are cut out and then the test piece with the
backside upward is smoothly fastened to the clamp of internal diameter 4.4 cm without wrinkling
and loosing. The force N when the test piece is broken down by a pushing rod at a pressing speed
of 10 cm/min is measured. The pushing rod has t